# stability of cellular patterns in directional solidification

Post on 09-Apr-2017

214 views

Embed Size (px)

TRANSCRIPT

PHYSICAL REVIEW A VOLUME 42, NUMBER 8

Stability of cellular patterns in directional solidification

15 OCTOBER 1990

John D. Weeks* and Wim van SaarloostAT& T Bel/ Laboratories, Murray Hill, New Jersey 07974

(Received 19 July 1990)

Ideas from the theory of constitutional supercooling, as well as an approximate linear stabilityanalysis for small wavelength perturbations, lead to a simple stability criterion for the periodiccellular patterns seen in the directional solidification of alloys with small partition coefficient.There is good qualitative agreement with the limited experimental data available in the cellularregime. This criterion suggests that solutions found by using the analogy between directionalsolidification and Saffman-Taylor fingers may be unstable.

hu;cos8 ID(n Vu); (2)

u; 1 z;/lT du@. , (3)

Recent analytical and numerical work has shown thatthe equations describing the directional solidification'(DS) of a binary mixture admit a continuous family ofperiodic steady-state cellular solutions with varying wave-lengths k. However, a steady-state analysis alone cangive no information about the stability of these solutions,and hence their relevance for real experiments. In this pa-per we present an approximate stability analysis that inmany cases will allow one to determine whether a givensteady-state solution is likely to be stable. The simplestprediction is based on ideas from the theory of constitu-tional supercooling, 's and we refer to it as the local con-stitutional supercooling (LCS) criterion. The LCS cri-terion relates the positions of the tips of stable periodiccellular arrays in the experimental cell to the pulling ve-locity V, and its predictions can easily be checked experi-mentally. A more general, but still approximate, linearstability analysis for arrays of cellular patterns suggeststhat in many cases corrections to the LCS criterion shouldbe small.

Equations similar to the LCS criterion have in fact beenused before, particularly in the dendritic regime found atstill higher pulling velocity, or smaller temperature gra-dient. However, the earlier derivations relied on some-what ad hoc matching arguments, and they attempted topredict a unique pattern spacing for a given set of experi-mental conditions, rather than determine which membersof a family of solutions might be stable. To ourknowledge, the derivation and interpretation of the LCScriterion and its corrections in terms of stability concepts,and its particular relevance in the cellular regime has notbeen realized before.

We consider the standard one-sided solutal model, '

where solidification is assumed to occur as matter in a thincell is pulled through a fixed linear temperature gradient,and impurity diffusion in the solid is ignored. The steady-state equations for DS in two dimensions in a frame mov-ing at velocity Vcan be written as'

1 Bu

az

where, using Eq. (3),

au; = u; u,'=1 (1 k)(z;/&T+do~) . (4)

which denotes the boundary of the stable single-phase re-gion in a modified phase diagram where the abscissa is thereduced concentration field u and the ordinate is the posi-tion z in the cell (by assumption linearly related to thetemperature T).

We note that in almost all cases, the curvature at thetips of experimentally relevant cellular patterns is smallenough that the term dux in (3) represents only a verysmall correction. '" (This will be discussed more quanti-tatively later. ) This suggests that we can think of the re-gion near the tips as locally planar, and use some of thesame stability ideas there that are used to examine thestability of the initial planar interface. The simplest ap-proximation leads directly to the LCS criterion.

Here do is the chemical capillary length, lT the thermallength, /D =D/ V a diffusion length, a' the interface curva-ture, and 8 the angle between the interface normal n andthe growth direction, taken parallel to the z axis. ' A sub-script i denotes a quantity evaluated at the interface, andthe superscript s denotes the solid phase. The dimension-less field u =(e c )/hen measures the impurity concen-tration c in the liquid relative to that far ahead of the in-terface c . It is normalized by the width of the planartwo-phase region, hco =co co =co(1 k), with k thepartition coefficient and co the concentration at the planarsteady-state interface. Global conservation of impuritiesthen fixes the location of the steady-state planar interfacein the cell such that c =kco, or equivalently,uu duo 1. This defines the origin z =0 of our coordi-nate system.

Equation (2) expresses local conservation of impuritiesas the interface advances, with hu; in (4) the "impuritysurplus" rejected at the interface. For materials withsmall partition coefficient k, we see that h, u; has asignificant dependence on the position z; in the cell. Thiswill play an important role in what follows.

Equation (3) takes account of surface-tension effectsand imposes local equilibrium at the interface. For planarinterfaces with ~ 0, it describes the liquidus line

(5)

5056 1990 The American Physical Society

STABILITY OF CELLULAR PAL IERNS IN DIRECTIONAL. . . 5057

To begin the analysis, let us review the theory of consti-tutional supercooling (CS) for the planar interface. 'The basic idea is that in the steady state we can apply theconcept of local thermodynamic equilibrium to the meltjust in front of the moving planar interface. The interfaceis supposed to remain stable as long as the impurity con-centration in the melt just in front lies in the stablesingle-phase region as determined from the phase dia-gram. Since we assume local equilibrium at the interfacefrom (3), the CS stability criterion reduces to the follow-ing requirement. The (dynamical) gradient ~du/dz ~;

d u;/lp determined from the boundary condition (2)must not exceed the liquidus slope ~duL/dz

~I/lr in (5).

This criterion can be reexpressed as

veau; ~1,where we define the standard dimensionless control pa-rameter ' v = ir/lD. Note that v is directly proportional tothe velocity V.

The usual CS prediction vc 1 for the stability limitof the plane' follows from (6) where we note that globalconservation requirements force the plane to be located atz; 0, where hu; 1. This criterion is surprisingly accu-rate, given the simplicity of the CS argument. For ma-terials with small k, a linear stability analysis (see below)predicts only small changes in the critical value of v, i.e.,~c= 1.

However, the arguments leading to (6) seem nearly asplausible as before when applied locally to the melt infront of the tips of certain (nonplanar) patterns, providedthat the curvature corrections in Eq. (3) are small, andthat k is reasonably small, e.g., k 50.2. In particular, weneed to use only the boundary conditions (2) and (3) andthe local symmetry in the tip region (nearly planar, with8, 0) to arrive at (6), with hu; h,u the impuritysurplus at the tip. When curvature corrections to du& from(4) are small, Eq. (6) can be reexpressed as

g, = (v 1)(1 k)z, /iD ~ 0 .Equation (7) predicts that the tip position z, of stable pat-terns with v & 1 must move up in the cell, relative to theplanar position at z 0, until the smaller impurity surplushu, allows (6) or (7) to hold true. It is natural to conjec-ture that the operating point in real experiments should beclose to the one that requires the least forward motion,i.e., the re~ion where g, =0. We refer to this as the LCScriterion. '

Of course, this argument is only suggestive. The CScondition (6) is not exact, even for the plane at z =0. It iseasy to see that corrections to the LCS picture must surelybe taken into account at large v & 1/k (usually in the den-dritic regime), since (7) would then predict an unphysical"concentration deficit" at the tip with u, & 0.

To determine the nature of the corrections to LCS, weextend the usual planar stability analysis' to the casewhere the wavelength of interface perturbations is smallcompared to A, , the wavelength of the (steady-state)profile z; (x). Representing the perturbed interface by

zf(x, t) z;(x)+zz exp(iqx+tot),

(8'u/8x '),co p2 +

ur

p (pv/p I+k)(veau, 1 (v l)crq ]Qt

(8)

Here p=A, /2lD is the Peclet number, which relates thescale of the pattern to the diffusion length, pv satisfiespv(pv p) q 2, and

ks 4 vdplD0g 9

k (v 1)

where X, is the (lower) neutral stability wavelength forthe plane in the limit as k 0. cr provides a measure ofthe importance of surface-tension corrections due to thecurvature of the interface. Experimental values for a areusually very small. ""3We note that (8) reduces to thestandard result for the plane, ' where hu, duo 1, and(r1 u/8x ), 0. The expression in (9) for A,, then followsfrom (8) if we set k 0 and solve for the associated wavevector q, giving co 0.

In general, for small k, the first term on the right-handside of (8) is small, and important only in a small regionof v very near threshold. The quantity (8 u/8x )& ap-pearing in the second term on the right in (8) is negative(stabilizing) and numerical calculations indicate that ittoo is often small in magnitude. '

We can then obtain the LCS criterion from (8) byneglecting both these terms as well as all terms propor-tional to o, ' requiring that a stable solution with to ~ 0results. This derivation makes it clear that the LCS con-dition g, =0 gives an upper bound to the distance that thetips of patterns have to move to achieve stability, since allterms omitted in (8) are negative (stabilizing). Correc-tions due to the curvature of the interface are more impor-tant at large v, since they are proportional to (v 1)~.Indeed, for very large v in the dendritic regime, the tipsmove up very close to the line z 1~. The stability is thend

Recommended